**HAL Id: hal-02348316**

**https://hal.archives-ouvertes.fr/hal-02348316**

### Submitted on 5 Nov 2019

**HAL**

### is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

### L’archive ouverte pluridisciplinaire

**HAL, est**

### destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

**Photo-induced phase transitions in ferroelectrics**

### Charles Paillard, Engin Torun, Ludger Wirtz, Laurent Bellaïche

**To cite this version:**

### Charles Paillard, Engin Torun, Ludger Wirtz, Laurent Bellaïche. Photo-induced phase transi- tions in ferroelectrics. Physical Review Letters, American Physical Society, 2019, 123, pp.087601.

### �10.1103/PhysRevLett.123.087601�. �hal-02348316�

Charles Paillard,^{1, 2} Engin Torun,^{3} Ludger Wirtz,^{3} Jorge ´I˜niguez,^{4, 3} and Laurent Bellaiche^{1}

2

1Department of Physics and Institute for Nanoscience and Engineering,

3

University of Arkansas, Fayetteville, Arkansas 72701, USA

4

2Laboratoire Structures, Propri´et´es et Mod´elisation des Solides, CentraleSup´elec,

5

UMR CNRS 8580, Universit´e Paris-Saclay, 91190 Gif-sur-Yvette, France^{∗}

6

3Physics and Materials Science Research Unit, University of Luxembourg,

7

162a avenue de la Fa¨ıencerie, L-1511 Luxembourg, Luxembourg

8

4Materials Research and Technology Department,

9

Luxembourg Institute of Science and Technology (LIST),

10

Avenue des Hauts-Fourneaux 5, L-4362 Esch/Alzette, Luxembourg

11

Ferroic materials naturally exhibit a rich number of functionalities, which often arise from ther- mally, chemically or mechanically induced symmetry breakings or phase transitions. Based on Density Functional Calculations, we demonstrate here that light can drive phase transitions as well in ferroelectric materials such as the perovskite oxides lead titanate and barium titanate. Phonon analysis and total energy calculations reveal that the polarization tends to vanish under illumina- tion, to favor the emergence of non-polar phases, potentially antiferroelectric, and exhibiting a tilt of the oxygen octahedra. Strategies to tailor photo-induced phases based on phonon instabilities in the electronic ground state are also discussed.

Ferroelectric materials possess a spontaneous electric

12

polarization that is switchable by electric fields. Active

13

research in bandgap engineering [1] and unconventional

14

photovoltaic mechanisms [2–4] have prompted perovskite

15

oxide ferroelectrics as potential light absorbers to con-

16

vert light into electric [5], mechanical [6–8] or chemi-

17

cal energy [9], or for optical memory writing [10] and

18

non-destructive reading [11]. Numerous works focused

19

on the photo-induced deformation of the unit cell with-

20

out apparent symmetry breaking [8]. However, a recent

21

experimental work hinted at possible structural phase

22

transitions occurring in ferroelectric BaTiO_{3} nanowires

23

under illumination [12]. Using first-principles calcula-

24

tions, we show that photo-induced phase transitions are

25

indeed possible in ferroelectrics such as barium and lead

26

titanates. In both cases, transitions to non-polar phases

27

are predicted. Furthermore, material engineering strate-

28

gies based on competing lattice instabilities are suggested

29

to tailor the critical concentration of photo-induced car-

30

riers at which the transition occurs, thus opening the

31

way to a rational design of materials exhibiting specific

32

properties under illumination.

33

ABO3perovskite oxides are versatile materials exhibit-

34

ing a wide range of properties (magnetism, polar distor-

35

tions, etc.). Their high symmetry reference structure (see

36

Fig. 1) is cubic with theBcation enclosed in an octahe-

37

dral cage of oxygens at the center, and theAcation at the

38

edges of the cube. Simple atomic displacement patterns

39

– e.g. as the octahedra tilts or electric dipoles sketched

40

in Fig. 1 – make it possible to obtain various symme-

41

try breakings and control the materials properties. For

42

convenience, here we denote the most relevant of such

43

distortions using a generalized and simplified Glazer no-

44

tation [13] αβγ/u^{α}^{0}v^{β}^{0}w^{γ}^{0}, which is introduced in the

45

caption of Fig. 1.

46

Among perovskite oxides, barium titanate (BTO) and

47

lead titanate (PTO) are prototypical ferroelectric mate-

48

rials. They exhibit a number of phases [14, 15] associated

49

with lattice instabilities of the reference cubic phase [16].

50

The transitions between phases are commonly driven by

51

temperature [14, 15], pressure [17–19] or static electric

52

fields [20]. Here, we demonstrate that light can also act

53

as a knob to control the crystal symmetry. Optical ma-

54

nipulation of ferroic materials has mainly focused on the

55

transient manipulation of the ferroic order parameter,

56

relying on non-thermalized photoexcited carriers [21] or

57

strong anharmonic phonon couplings [22]. In contrast, we

58

presently describe the emergence of new phases caused by

59

modified lattice instabilities in the presence of thermal-

60

ized photo-excited carriers,i.e. the electrons lying at the

61

bottom of the conduction band (CB) and the equal num-

62

ber of holes sitting at the top of the valence band (VB)

63

of a semiconductor during illumination. To this end, we

64

usedab-initio calculations, detailed in the next section,

65

before examining the cases of barium and lead titanate

66

respectively. Finally, we discuss the origin of this phe-

67

nomenon and test design strategies for the engineering of

68

photo-induced phase transitions in ferroelectrics.

69

We performed Density Functional Theory (DFT) cal-

70

culations using the Abinit package software [23], with

71

the Projector Augmented Wave (PAW) method [24, 25].

72

We employ a 2×2×2 supercell (with respect to the 5-

73

atom pseudo-cubic perovskite cell) containing 40 atoms.

74

Thek-point mesh used was a Γ-centered 8×8×8 grid;

75

the plane-wave cut-off was 35 Ha. A Fermi-Dirac distri-

76

bution with 0.1 eV smearing was used to populate the

77

electronic states. The electronic density was considered

78

converged when the difference in the calculated forces be-

79

tween two Self-Consistent Field (SCF) steps was smaller

80

than 10^{−8} Ha.Bohr^{−1}. The structural relaxation was

81

2

*000/000*

*000/00w*^{+}

*00+/000*
*00-/000*

*000/u*^{+}*u*^{+}*0** ^{-}*
polar displacements

Tilts

FIG. 1. Sketch of a 2×2×2 supercell in the paraelectric cubic
reference structure 000/000. A and B cations are in black and
blue, oxygens in red. The symmetry of a phase is denoted by
(i)its oxygen octahedra tilt patternαβγ, whereα,βandγare
either 0 (no tilt), ”+” (in-phase tilt) or ”−” (antiphase tilt)
and represent whether the oxygen octahedra tilts around the
first, second and third pseudocubic axis, respectively. Simi-
larly, we denote the electric dipole pattern using a Glazer-like
notationu^{α}^{0}v^{β}^{0}w^{γ}^{0}, in whichu, v, wrepresent the magnitude
of the dipole inside the perovskite 5-atom cell, andα^{0}, β^{0}and
γ^{0}describes whether dipole vectors [uvw] are aligned parallel
(”+”) or antiparallel (”−”) when moving by one perovskite
5-atom cell along the first, second and third pseudocubic di-
rection. Typical polar (000/00w^{+}), antipolar (000/u^{+}u^{+}0^{−}),
in-phase (00c^{+}/000) and antiphase tilt (00c^{−}/000) displace-
ment patterns are depicted using arrows.

stopped when all the forces on the atoms were smaller

82

than 5 ×10^{−7} Ha.Bohr^{−1} and all components of the

83

stress tensor smaller than 0.1 MPa. BTO was described

84

using the PBESol [26] exchange-correlation functional,

85

while the Local Density Approximation [27, 28] was em-

86

ployed to treat PTO. Photo-excited thermalized carriers

87

are mimicked using Fermi-Dirac distribution with two

88

quasi-Fermi levels µe and µh, as commonly used to de-

89

scribe photovoltaic effects in, for instance, p−n junc-

90

tions [29]. As a result, during our DFT calculations, the

91

density is self-consistently converged under the constraint

92

of having ne=nph (and nh =nph) electrons (holes) in

93

the CB (VB). In other words, at each Self-Consistent

94

Field (SCF) iteration, the following system of equations

95

nh= X

i≤Nv

X

k,σ

wk[1−f(εik,σ, µh)], (1) ne= X

i>Nv

X

k,σ

wkf(εik,σ, µe), (2)
is solved for µ_{e} and µ_{h} using a bisection algorithm.

96

In the above equation, wk is the weight of k-point k,

97

f(εik, µ) is the occupation number (Fermi-Dirac distri-

98

bution) of state with eigenvalueεik;σ denotes the spin.

99

Nv is the index of the highest valence band. We assume

100

that there is no closing of the gap during our constrained

101

DFT calculations, which is in practice observed for the

102

concentrations of photo-excited carrier pairsn_{ph} consid-

103

ered in this work.

104

Note that all structures considered in this work were

105

geometrically relaxed under the photo-excitation con-

106

straint mentioned above. The criteria for convergence

107

of the structural degrees of freedom are set to be the

108

same as in electronic ground state calculations.

109

Phonon calculations using the Phonopy package [30]

110

were performed in the dark and under excitation on the

111

cubic perovskite oxides using a 2×2×2 supercell after

112

the system was structurally relaxed. No analytic cor-

113

rection, and thus no LO-TO splitting was considered, as

114

the required Born effective charges cannot be calculated

115

in photo-excited cases.

116

We first calculated the phonon band structure of cu-

117

bic BTO in Figs. (2.a-d) for different concentrations of

118

photoexcited carriers nph. In the dark (nph = 0 e/f.u.,

119

Fig. (2.a)), the phonon dispersion exhibits imaginary

120

(negative in the figure) frequency modes characteris-

121

tic of lattice instabilities. The main instability, at Γ,

122

is responsible for the emergence of the polar order in

123

BTO [16], which goes from a high temperature cubic

124

000/000 structure to a ferroelectric tetragonal 000/00w^{+}

125

phase below∼393 K, then to an orthorhombic structure

126

000/0v^{+}v^{+} below ∼280-270 K and finally to a rhombo-

127

hedral 000/u^{+}u^{+}u^{+} phase below ∼183 K [14]. Upon

128

increasing the number of photo-excited carrier pairs to

129

nph = 0.05 e/f.u. (in Fig. (2.b)), the frequencies of un-

130

stable modes along theX−M−Γ path get closer to real

131

(positive) values, the ferroelectric soft optical mode at Γ

132

becoming less unstable. Furthermore, fornph≥0.1 e/f.u.

133

(Figs. (2.c-d)) the cubic phase no longer exhibits unstable

134

phonon modes and isdynamically stable!

135

We calculated the energy (see Fig. (3.a)) of the four

136

phases naturally occurring in bulk BTO, 000/000 (green

137

squares), 000/00w^{+} (blue diamonds), 000/0v^{+}v^{+} (vio-

138

let triangles) and 000/u^{+}u^{+}u^{+} (ground state at 0 K in

139

dark conditions, black dashed baseline). The rhombohe-

140

dral phase has the lowest energy for low concentrations of

141

photo-excited carriers (up to≈0.0375 e/f.u.), while the

142

tetragonal phase is slightly more stable at intermediate

143

concentrations (nph≈0.0375−0.1 e/f.u.). When the cu-

144

bic phase is dynamically stable (nph>0.1 e/f.u.), we find

145

accordingly that 000/000 is the lowest-energy structure,

146

which is confirmed by the disappearance of polar atomic

147

displacements and the cell shape distortions of all con-

148

sidered phases (see Supplementary Material [31]). The

149

predicted transition towards the 000/000 phase is con-

150

sistent with the experimental observation, in BTO, of a

151

downward shift of the Curie temperature under illumina-

152

tion [32]. Besides, the flattening of the energy landscape

153

around 0.03 e/f.u. (≈5×10^{20}e.cm^{−3}) may be accompa-

154

nied by a monoclinic phase transition (see Supplemental

155

Γ *X* *R M* Γ *R* *X M* Γ
0

10 20

¯hω(THz)

Γ *X* *R M* Γ *R* *X M* Γ
0

10 20

¯hω(THz)

Γ *X* *R M* Γ *R* *X M* Γ
0

10 20

¯hω(THz)

Γ *X* *R M* Γ *R* *X M* Γ
0

10 20

¯hω(THz)

## BT O

*n*

_{ph}### (e/f.u.)

Γ *X* *R M* Γ *R* *X M* Γ

*−5*
0
5
10
15
20
25

¯hω(THz)

Γ *X* *R M* Γ *R* *X M* Γ

*−5*
0
5
10
15
20
25

¯hω(THz)

Γ *X* *R M* Γ *R* *X M* Γ

*−5*
0
5
10
15
20
25

¯hω(THz)

Γ *X* *R M* Γ *R* *X M* Γ

*−5*
0
5
10
15
20
25

¯hω(THz)

## PT O

### (a) (b) (c) (d)

### (e) (f) (g) (h)

### 0.00 0.05 0.10 0.15

FIG. 2. (a-d) Phonon band structure in paraelectric cubic BTO and (e-h) PTO for different concentrations of photoexcited carrier pairsnph = 0.00 e/f.u. (a & e), nph = 0.05 e/f.u. (b & f),nph= 0.10 e/f.u. (c & g) andnph= 0.15 e/f.u. (d & h).

The polar Γ dominant instability in BTO becomes stabilized (i.e. positive and real frequency) fornph≥0.10 e/f.u., as shown in (c) and (d). In PTO, the polar instability at Γ is replaced by a non-polar tilted instability atM andR.

Material [31]). We note that such a critical concentration

156

would match recent observations of a monoclinic phase

157

in BTO nanowires under illumination [12, 33].

158

PTO exhibits a single transition from the non-polar

159

cubic 000/000 phase to the ferroelectric tetragonal

160

000/00w^{+} structure below 765 K [15]. The phonon dis-

161

persion of the cubic phase fornph= 0 e/f.u. (Fig. (2.e))

162

exhibits one main polar instability at Γ, but also unstable

163

modes at theRandM points associated with octahedra

164

tilting 00−and 00+, respectively. The strength of the po-

165

lar instability at Γ decreases with increasing the number

166

of photo-excited carriers (see Figs. (2.e-h)) as in BTO.

167

However, it never totally disappears, indicating that fer-

168

roelectricity in PTO is more robust against photocarrier

169

generation. In contrast, the strengths of the tilting in-

170

stabilities at R and M are slightly enhanced, and they

171

become dominant forn_{ph} ≥0.1 (Figs. (2.g-h)), suggest-

172

ing a transition from a polar to a non-polar structure

173

with oxygen tilts under illumination.

174

Hence, we compute the energies of several prototypi-

175

cal phases upon illumination, as shown in Fig. (3.b). The

176

ferroelectric 000/00w^{+} phase, which is the ground state

177

in dark conditions, is the black dashed baseline, while the

178

cubic phase is plotted as green squares. We also plot a

179

rhombohedral polar− − −/u^{+}u^{+}u^{+} structure (navy cir-

180

cles) and its non-polar counterpart, a− − −/000 (navy

181

diamonds). We consider as well an orthorhombic phase

182

(violet triangles) with the − −0/u^{−}u¯^{−}0^{−} antipolar dis-

183

placement pattern [34]. A 00c^{−}/000 non-polar tetrago-

184

nal phase is also calculated (gold triangles). According to

185

Fig. (3.b), the ferroelectric 000/00w^{+} phase is the most

186

stable up tonph≈0.125 e/f.u., the non-polar phase with

187

tilts becoming dominant beyond that point. Overall, the

188

antipolar − −0/u^{−}u¯^{−}0^{−} phase is slightly more favor-

189

able (by 0.2-0.3 meV/f.u.) than the− − −/000 phase for

190

nph ≥0.125 e/f.u. Because of this small energy differ-

191

ence, it is impossible to predict with certainty the sym-

192

metry of PTO at large concentrations of photo-excited

193

carriers, and we can only reckon that this should be a

194

phase with oxygen tilts.

195

Unlike BTO, the polar atomic distortion in the

196

000/00w^{+} phase remains rather large under photo-

197

excitation (see Supplementary Material [31]). Moreover,

198

both the antipolar displacement (for the− −0/u^{−}u¯^{−}0^{−}

199

phase) and the tilt angle (for − − −/000 and − −

200

0/u^{−}u¯^{−}0^{−}) increase withnph. In contrast, the polar dis-

201

placements of the− − −/u^{+}u^{+}u^{+} phase disappear with

202

increasingnph, and it thus collapses into the− − −/000

203

phase, confirming that tilts and polarization are com-

204

peting order parameters in PTO [35, 36], illumination

205

tipping the balance towards the former.

206

Furthermore, calculations of minimum energy tran-

207

sition paths between phases (see Supplementary Mate-

208

rial [31]) show that − −0/u^{−}u¯^{−}0^{−} and − − −/000 are

209

unstable in the dark; however, the 000/00w^{+} phase re-

210

mains metastable under illumination, drawing the pic-

211

ture of a first-order light-induced transition in PTO.

212

The large concentration of 0.125 e/f.u. needed to

213

destabilize the 000/00w^{+} phase in PTO is potentially

214

outside the reach of experiments, and certainly not de-

215

sirable for applications. We can try to improve this

216

situation by mixing PTO with an antiferrodistortive

217

4

0.00 0.05 0.10 0.15

*n**ph* (e/f.u.)
0

5 10 15

*E−E*000*/u*+*u*+*u*+(meV/f.u.)

000/0^{+}*v*^{+}*v*^{+}
000/000
000/00w^{+}

0.00 0.05 0.10 0.15

*n**ph* (e/f.u.)
0

20 40

*E−E*000*/*00*w*+(meV/f.u.)

000/000

*− − −**/000*

*− − −**/u*^{+}*u*^{+}*u*^{+}

*− −*0/u^{−}*u*¯* ^{−}*0

*00*

^{−}*−*

*/000*

0.00 0.05 0.10 0.15

*n** _{ph}* (e/f.u.)
0

5 10 15 20

*E−E**−−−**/u*+*u*+*u*+(meV/f.u.) ^{000/000}

*− − −**/000*

*− −*0/u^{−}*u*¯* ^{−}*0

*000/0*

^{−}^{+}0

^{+}

*w*

^{+}00

*−*

*/000*

## (a)

## (b)

## (c)

FIG. 3. (a) Energy of different phases in BTO with respect
to the 000/u^{+}u^{+}u^{+} structure (dashed dark line), which is
the ground state in the dark. The tetragonal 000/00w^{+} and
then the cubic 000 phase become more energetically favor-
able. (b) Energy of different phases in PTO with respect
to the 000/00w^{+} structure (dashed dark line), which is the
ground state in the dark, showing that non-polar antiferrodis-
tortive phases become more stable at large concentration of
photo-excited carriers. (c) Energy of different phases in PSTO
with respect to the rhombohedral − − −/u^{+}u^{+}u^{+} structure
(dashed dark line), which is the lowest energy phase consid-
ered when no carriers are excited.

material such as SrTiO_{3}, and form the solid solution

218

(Pb_{1/2}Sr_{1/2})TiO_{3} (PSTO) to favor the tilt instability

219

with respect to the polar one. As a proof of concept,

220

several phases of PSTO with rocksalt order were cal-

221

culated in Fig. (3.c). In particular, a polar rhombohe-

222

dral − − −/u^{+}u^{+}u^{+} phase (black dashed line) is the

223

ground state in the dark. The 000/00w^{+} (purple tri-

224

angles) and the high-symmetry cubic 000/000 phase (in

225

green squares) have increasing energy withnph. On the

226

contrary, the antipolar tilted phase− −0/u^{−}u¯^{−}0^{−} (light

227

blue triangles) becomes the most stable phase above

228

n_{ph} = 0.05 e/f.u., thus supporting the proposed design

229

strategy to reduce the critical concentration for the polar-

230

to-antipolar/antiferrodistortive transition.

231

From this work, it also becomes apparent that the fer-

232

roelectric instability can be hampered by the photogen-

233

eration of free carriers. Obviously, free carriers screen the

234

long-range Coulombic interaction responsible for the po-

235

lar order [37, 41], thus seemingly disfavoring polar phases

236

with respect to non-polar ones. This is consistent with

237

calculations [37, 41] and experiments [42] performed by

238

doping BTO with free electrons. The former predicted

239

the disappearance of the polar order in BTO at a concen-

240

tration of extra-electrons of≈0.1 e/f.u., which is exactly

241

the concentration of photo-excited carriers that stabilizes

242

the cubic phase in our calculations. We also note that the

243

destruction of the polar order in BTO and the large sta-

244

bility (and metastability) window of the 000/00w^{+}phase

245

in PTO are consistent with the doping calculations per-

246

formed in Ref. [37]. In addition, photoexcitation tends to

247

move electrons from O 2pstates to Tidstates, thus de-

248

stroying the covalent bonding that drives the ferroelectric

249

order [40] and favoring non-polar orders. Looking at the

250

evolution of interatomic force constants (IFCs; see Sup-

251

plementary Material [31]) under photoexcitation, shows

252

that(i)almost all IFCs are reduced in magnitude under

253

photoexcitation, and (ii) the most affected IFCs corre-

254

sponds to 4th nearest neighbors interaction,i.e. similar

255

atoms (Ti-Ti, O-O, etc.) interacting along the<100 >

256

cubic directions. This parallels the further stabilization

257

of the paraelectric phase under photoexcitation in the

258

incipient ferroelectric PbTe, which results from screen-

259

ing of the long-range Coulomb interactions by the redis-

260

tributed photoexcited carriers along the<100 >cubic

261

directions [38]. From the evidence presented here, as well

262

as in other works involving doping and photoexcited cal-

263

culations [37, 38], electrostatic screening by photoexcited

264

carriers appears as a universal mechanism for ”dipole-

265

dipole driven” ferroelectric materials such as BTO [39].

266

In addition, the volume of most phases decreases with

267

increasing concentration of excited carriers in both BTO

268

and PTO, except that of the cubic 000/000 phase, which

269

increases instead (see Supplementary Material [31]). In-

270

terestingly, the decrease of volume of the polar phases

271

is consistent with the disappearance of the polar order,

272

and is reminiscent of the well-known [17–19] effect of hy-

273

drostatic compression; yet, the volume increase of the

274

cubic phase under illumination should in principle favor

275

the polar instabilities. Hence, our results suggest that the

276

behavior of the polar distortion upon illumination cannot

277

be understood solely in terms of a photo-induced volume

278

change [43], and that screening effects play a central role.

279

There are, however, potential limitations of this work,

280

since DFT is known to underestimate the quasi-particle

281

bandgap. Furthermore, excitonic effects are described

282

within a mean-field approximation using constrained

283

DFT to mimic excited states occupations. First, we per-

284

formedG_{0}W_{0}[44] calculations with the Yambo [45] pack-

285

age - using DFT input from Quantum Espresso [46, 47]

286

- in order to accurately describe the conduction and va-

287

lence bands (see Supplementary Material [31]). The cor-

288

rected band structure is overall not altered, except for

289

an almost rigid upshift of the conduction bands. This

290

shift slightly depends on the studied phase (with differ-

291

ences smaller than 100 meV between phases). The shift is

292

smaller for non-polar phases, therefore facilitating further

293

the light-induced transitions towards such latter states.

294

For BTO, we checked the robustness of our conclu-

295

sions by performing calculations of zone center phonons

296

of the cubic phase with hybrid DFT. We compare calcu-

297

lations performed with the semi-local PBEsol functional

298

and the hybrid HSEsol [48] functional. Both functionals

299

give similar lattice constants and similar frequency for

300

the imaginary frequency of the soft ferroelectric mode,

301

even though the band gaps are quite different (1.8 eV for

302

PBEsol and 3.4 eV, close to the GW value, for HSEsol).

303

Despite the very different band gaps, the phonon frequen-

304

cies as a function of the excited charge density evolve sim-

305

ilarly: we observe a stabilization of the soft mode at an

306

excited charge density of 0.09 electron per formula unit

307

(see Supplementary Material [31]). Hence, although our

308

DFT-based description may slightly alter the critical con-

309

centrations at which transitions occur, the present qual-

310

itative behavior should be correct, especially given our

311

results in Fig. 2 for the dynamical lattice instabilities of

312

theparaelectric cubic state.

313

At last, let us discuss the possibility of having photo-

314

induced phase transitions to (small self-trapped, or ST)

315

polaronic states. Recent (doping) calculations have

316

shown that ST holes were unlikely in PTO [49, 50], but

317

could potentially be stabilized in cubic BTO [49]. In

318

order to check the appearance of polaronic states, we

319

ran calculations in BaTiO3 under photoexcitation with

320

n_{ph} = 0.075 e/f.u. andn_{ph} = 0.150 e/f.u (with no sym-

321

metry). No trace of polaronic states was found.

322

In conclusion, we have shown that light absorption is

323

a viable route to switch on/off specific lattice instabili-

324

ties in complex materials such as ferroelectric perovskite

325

oxides. Via first-principles calculations we have demon-

326

strated the microscopic mechanism leading to a light-

327

controlled stabilization of the cubic phase in BTO but

328

not in PTO. The calculations are a promising tool to en-

329

gineer and optimize such light-triggered transformations,

330

suggesting strategies for their practical realization in suit-

331

ably chosen materials. The results presented in this work

332

could offer a route to design light-controlled memory, by

333

accessing light-induced metastable states (see Fig. 4 in

334

the Supplemental Material [31] and related discussion).

335

C. P. and L. B. thank the ARO grant W911NF-

336

16-1-0227. We also acknowledge support from the

337

National Research Fund, Luxembourg through project

338

INTER/ANR/13/20/NANOTMD (E. T. and L. W.)

339

and the intermobility program (Grant No. 15/9890527

340

Greenox, J. I. and L. B.). C. P. thanks the AHPCC and a

341

DoD challenge grant for use of computing resources. We

342

thank B. Dkhil and P. Ruello for interesting discussions.

343

∗ charles.paillard@centralesupelec.fr

344

[1] I. Grinberg, D. V. West, M. Torres, G. Gou, D. M. Stein,

345

L. Wu, G. Chen, E. M. Gallo, A. R. Akbashev, P. K.

346

Davies, J. E. Spannier, A. M. Rappe, Nature 503, 509

347

(2013).

348

[2] B. I. Sturman, V. M. Fridkin, The Photovoltaic and

349

Photorefractive Effects in Noncentrosymmetric Materi-

350

als, Gordon and Breach Science Publishers (1992).

351

[3] L. Z. Tan, F. Zheng, S. M. Young, F. M. Wang, S. Liu, A.

352

M. Rappe,npj Computational Materials2, 16026 (2016).

353

[4] C. Paillard, X. Bai, I. C. Infante, M. Guennou, G. Gen-

354

este, M. Alexe, J. Kreisel, B. Dkhil,Advanced Materials

355

28, 5153 (2016).

356

[5] R. Nechache, C. Harnagea, S. Li, L. Cardenas, J.

357

Chakrabartty, F. Rosei,Nature Photonics9, 61 (2014).

358

[6] B. Kundys, M., Viret, D., Colson, D. O. Kundys,Nature

359

Materials9, 803 (2010).

360

[7] M. Lejman, G. Vaudel, I. C. Infante, P. Gemeiner, V. E.

361

Gusev, B. Dkhil, P. Ruello,Nat. Commun.5, 4301 (2014).

362

[8] B. Kundys,Applied Physics Reviews 2, 011301 (2015).

363

[9] Y. Cui, J., Briscoe, S. Dunn,Chemistry of Materials25,

364

4215 (2013).

365

[10] V. Iurchuk, D. Schick, J. Bran, D. Colson, A. Forget, D.

366

Halley, A. Koc, M. Reinhardt, C. Kwamen, N. A. Morley,

367

M. Bargheer, M. Viret, R. Gumeniuk, G. Schmerber, B.

368

Doudin, B. Kundys,Physical Review Letters117, 107403

369

(2016).

370

[11] R. Guo, L. You, Y. Zhou, Z. S. Lim, X. Zou, L. Chen,

371

R. Ramesh, J. Wang, Nature Communications 4, 1990

372

(2013).

373

[12] Y.-H. Kuo, S. Nah, K. He, T. Hu, A. M. Lindenberg,

374

Journal of Material Chemistry C 5, 1522 (2017).

375

[13] A. M. Glazer,Acta Crystallographica B28, 3384 (1972).

376

[14] G. H. Kwei, A. C. Lawson, S. J. L. Billinge, S. W.

377

Cheong, S. W. The Journal of Physical Chemistry 97,

378

2368 (1993).

379

[15] G. Shirane, S. Hoshino,Journal of the Physical Society

380

of Japan6, 265 (1951).

381

[16] P. Ghosez, E. Cockayne, U. V. Waghmare, K. M. Rabe,

382

Physical Review B 60, 836 (1999).

383

[17] I. A. Kornev, L. Bellaiche, P. Bouvier, P.-E. Janolin,

384

B. Dkhil, J. Kreisel,Physical Review Letters 95, 196804

385

(2005).

386

[18] P.-E. Janolin, P. Bouvier, J. Kreisel, P. A. Thomas, I.

387

A. Kornev, L. Bellaiche, W. Crichton, M. Hanfland, B.

388

Dkhil,Physical Review Letters 101, 237601 (2008).

389

[19] M. Ahart, M. Somayazulu, R. E. Cohen, P. Ganesh, P.

390

Dera, H.-k. Mao, R. J. Hemley, Y. Ren, P. Liermann &

391

Z. Wu,Nature451, 545 (2008).

392

[20] H. Moriwakeet al.,J. Appl. Phys.119, 064102 (2016).

393

[21] A. Kirilyuk, A. V. Kimel, T. Rasing, Rev. Mod. Phys.

394

6 82, 2731 (2010).

395

[22] A. Subedi,Phys. Rev. B 92, 214303 (2015)

396

[23] X. Gonzeet al. Computational Physics Communications

397

180, 2582 (2009).

398

[24] P. E. Bl¨ochl,Physical Review B 50, 17953 (1994).

399

[25] M. Torrent, F. Jollet, F. Bottin, G. Z´erah, X. Gonze,

400

Computational Material Science 42, 337 (2008).

401

[26] J. P. Perdew, A. Ruzsinszky, G. I. Csonka, O. A. Vydrov,

402

G. E. Scuseria, L. A. Constantin, X. Zhou, K. Burke,

403

Physics Review Letters 100, 136406 (2008).

404

[27] W. Kohn, L. J. Sham, Physical Review 140, A1133

405

(1965)

406

[28] J. P. Perdew, Y. Wang, Physical Review B 45, 13244

407

(1992).

408

[29] P. W¨urfel, U. W¨urfel,Physics of Solar Cells: From Basic

409

Principles to Advanced Concepts, Wiley-VCH (2009).

410

[30] A. Togo, I. Tanaka,Scripta Materialia 108, 1 (2015).

411

[31] See Supplementary Material at ... for more details which

412

includes Refs. [12, 14, 17–19, 37, 42, 43, 45–48, 51?

413

? –58]. We detail the symmetry and atomic displace-

414

ment evolution under excitation of carriers; Nudge Elas-

415

tic Band calculations show that the transition is likely

416

to be first order and that the non-polar phase are not

417

metastable, but rather unstable; we discuss the occur-

418

rence of a monoclinic phase in BaTiO3; Volume changes

419

under illumination are compared with hydrostatic pres-

420

sure results from the literature. The evolution of Inter-

421

atomic Force Constants is also depicted. Finally, via the

422

GW-approximation and hybrid DFT calculations, we dis-

423

cuss the relevance of many-body effects for the photo-

424

iduced stabilization of the cubic phase.

425

[32] L. Belyaev, V. M. Fridkin, A. A. Grekov, N. A. Kosono-

426

gov, A. I. Rodin,Le J. Phys. Colloq.33, C2-123 (1972).

427

[33] Pump-probe experiments on BiFeO3 in Ref. [7] estimate

428

nph ∼ 5×10^{19}e cm^{−3} with maximum used fluences

429

of ∼50µJ.cm^{−2}. In Ref. [12] (which observes a mono-

430

clinic phase in BaTiO3nanowires) fluences ranging up to

431

600µJ.cm^{−2} are used, which would correspond to a car-

432

rier concentration of ∼ ^{600}_{50}.5×10^{19} ≈6×10^{20}e cm^{−3}.

433

This order of magnitude matches the region where we

434

observed flattening of the energy landscape in Fig. 3a

435

(around the 000/u^{+}u^{+}u^{+}to 000/00w^{+}transition) which

436

could potentially harbor a monoclinic phase as discussed

437

in the Supplementary Material [31].

438

[34] L. Bellaiche, J. ´I˜niguez, Physical Review B 88, 014104

439

(2013).

440

[35] I. A. Kornev, L. Bellaiche, P.-E. Janolin, B. Dkhil, E.

441

SuardPhysical Review Letters 97, 157601 (2006).

442

[36] J. C. Wojde l, P. Hermet, M. P. Ljungberg, P. Ghosez,

443

J. ´I˜niguez, Journal of Physics: Condensed Matter 25,

444

305401 (2013).

445

[37] H. J. Zhao, A. Filippetti, C. Escorihuela-Sayalero, P.

446

Delugas, E. Canadell, L. Bellaiche, V. Fiorentini, and

447

J. ´I˜niguez,Physical Review B 97, 054107 (2018).

448

[38] M.P. Jiang, M. Trigo, I. Savi´c, ´E. D. Murray, C. Bray,

449

J. Clark, T. Henighan, M. Kozina, M. Chollet, J. M.

450

Glownia, M. C. Hoffmann, D. Zhu, O. Delaire, A. F.

451

May, B. C. Sales, A. M. Lindenberg, P. Zalden, T. Sato,

452

R. Merlin, D. A. Reis,Nat. Commun.7, 12291 (2016).

453

[39] A. Filippetti, V. Fiorentini, F. Ricci, P. Delugas, J.

454

´I˜niguez,Nat. Commun.7, 11211 (2016).

455

[40] R. E. Cohen,Nature 358, 136 (1992).

456

[41] Y. Wang, X. Liu, J. D. Burton, S. S. Jaswal, E. Y. Tsym-

457

bal,Physical Review Letters 109, 247601 (2012).

458

[42] J. Fujiokaet al.,Scientific Reports5, 13207 (2015).

459

[43] C. Paillard, S. Prosandeev, L. Bellaiche,Physical Review

460

B 96, 045205 (2017).

461

[44] M. S. Hybertsen, S. G. Louie, Phys. Rev. B 34, 5390

462

(1986).

463

[45] Marini, A., Hogan, C., Gr¨uning, M. & Varsano, D.

464

Yambo: An ab initio tool for excited state calculations.

465

Comput. Phys. Commun.180, 1392–1403 (2009).

466

[46] Giannozzi, P.et al.QUANTUM ESPRESSO: a modular

467

and open-source software project for quantum simula-

468

tions of materials.J. Phys. Condens. Matter 21, 395502

469

(2009).

470

[47] Giannozzi, P.et al. Advanced capabilities for materials

471

modelling with Quantum ESPRESSO.J. Phys. Condens.

472

Matter 29, 465901 (2017).

473

[48] L. Schimka, J. Harl, G. Kresse, J. Chem. Phys. 134,

474

024116 (2011).

475

[49] P. Erhart, A. Klein, D. ˚Aberg, B. Sadigh,Phys. Rev. B

476

90, 035204 (2014).

477

[50] C. Paillard, G. Geneste, L. Bellaiche, B. Dkhil,J. Phys.

478

Condens. Matter 29, 485707 (2017).

479

[51] H. D. Megaw,Acta Crystallographica5, 739 (1952).

480

[52] E. Weinan, W. Ren, E. Vanden-Eijnden,J. Chem. Phys.

481

126, 164103 (2007).

482

[53] Z.-G. Ye, B. Noheda, M. Dong, D. E. Cox, G. Shirane,

483

Physical Review B 64, 184114 (2001).

484

[54] L. Bellaiche, A. Garc´ıa, D. Vanderbilt,Physical Review

485

Letters 84, 5427 (2000).

486

[55] D. Sangalli, A. Ferretti, H. Miranda, C. Attaccalite, I.

487

Marri, E. Cannuccia, P. Melo, M. Marsili, F. Paleari,

488

A. Marrazzo, G. Prandini, P. Bonf`a, M.O. Atambo, F.

489

Affinito, M. Palummo, A. Molina-S´anchez, C. Hogan, M.

490

Gr¨uning, D. Varsano, A. Marini, arXiv:1902.03837 [cond-

491

mat.mtrl-sci] (2019).

492

[56] C. Thomsen, H.T. Grahn, H.J. Maris, and J. Tauc,Phys.

493

Rev. B 34, 4129 (1986).

494

[57] R. Dovesi, A. Erba, R. Orlando, C. M. Zicovich-Wilson,

495

B. Civalleri, L. Maschio, M. Rerat, S. Casassa, J. Baima,

496

S. Salustro, B. Kirtman, WIREs Comput Mol Sci. 8,

497

e1360 (2018)

498

[58] G. Sophia, P. Baranek, C. Sarrazin, M. Rerat, R. Dovesi,

499

Phase Transitions: A Multinational Journal, 81, 1069-

500

1084 (2013).

501